| ||Format||Pages||Price|| |
|5||$43.00||  ADD TO CART|
|Hardcopy (shipping and handling)||5||$43.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$51.60||  ADD TO CART|
Significance and Use
5.1 Sandwich panel cores may change planar dimensions when heated. This phenomenon can be associated with the effects of heating upon the core material itself, as well as changes in core moisture content resulting from the heating cycle. It is prudent to know if this may be problematic with regard to the intended final part dimensions.
5.2 This test method provides a standard method of characterizing the dimensional stability of sandwich core materials for design properties, material specifications, research and development applications, and quality assurance.
5.3 Factors that influence dimensional stability of sandwich core materials and shall therefore be reported include the following: core material, methods of material fabrication, core geometry, core thickness, core thickness uniformity, cell wall thickness, specimen geometry, specimen preparation, heating and cooling environments (including temperatures and humidity levels), and specimen conditioning (both prior to and after heating).
1.1 This test method covers the determination of the sandwich core dimensional stability in the two plan dimensions.
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.2.1 Within the text, the inch-pound units are shown in brackets.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D5229/D5229M Test Method for Moisture Absorption Properties and Equilibrium Conditioning of Polymer Matrix Composite Materials
E122 Practice for Calculating Sample Size to Estimate, With Specified Precision, the Average for a Characteristic of a Lot or Process
ICS Number Code 83.120 (Reinforced plastics)
ASTM D6772 / D6772M-15, Standard Test Method for Dimensional Stability of Sandwich Core Materials, ASTM International, West Conshohocken, PA, 2015, www.astm.orgBack to Top